CARBON NANOTUBE AND GRAPHENE OXIDE BASED MEMBRANES
Aneela Sabir, Maria Wasim, Muhammad Shafiq, Tahir Jamil Department of Polymer Engineering and Technology, University of the Punjab, Lahore, Pakistan
1 MEMBRANE A membrane is regarded as a semipermeable barrier that allows certain species of a specific size to pass through it while blocking others, as illustrated in Fig. 1. The characteristics of membranes are what allow which species are to be filtered. Membrane science is a quickly growing field with real-time applications, including water purification and desalination. Research has been ongoing for developing a precise, cost-effective membrane, although the accuracy, precise ability, and cost-effectiveness can be dependent on the class of membrane used. However, until now, fabricating atomic-scale pores within membranes that allow the perfect retention of ions and molecules depending on their size is a challenging issue . Nanoscale Materials in Water Purification. https://doi.org/10.1016/B978-0-12-813926-4.00019-7 # 2019 Elsevier Inc. All rights reserved.
CHAPTER 14 CARBON NANOTUBE AND GRAPHENE OXIDE
FIG. 1 Schematic illustration of a membrane system.
2 CURRENT MEMBRANES Conventionally, membranes have been categorized into two types: polymeric [2–5] and inorganic membranes [6–8]. Based on their applicability, choosing which among them is the most ideal membrane type is difficult as they each have their own advantages and disadvantages. For example, polymeric membranes have shown excellent permeability, as well selectivity, but have limited resistance to high temperatures, solvents, and corrosive substances , whereas inorganic membranes, mostly composed of metals and ceramics, show superior thermal and mechanical stability, along with high mechanical and structural strength. However, these membranes have shown high selectivity at the expense of poor or limited permeability, which can deter their use for commercial-scale applications. Also, microporous silica-based membranes, which belong to the inorganic membrane class, have been employed for molecular sieving applications. The prime issue is fabricating a size-dependent filtration membrane with the precise control of pore size (in submicron range). However, the use of zeolite membranes, a type of inorganic membrane, has been fixing these issues to some extent. Zeolite-based membranes have shown stability at high temperatures, as well as a hydrophilic character and organophilic characteristics [10–13]. Zeolite membranes could be employed at the molecular scale but have some limitation, including their ion-exchange capability, solid acidity, adsorption, and the catalytic nature of zeolite. These limitations can act as properties for certain applications but forbid the use of zeolite as a neutral filler in membranes. It has also been shown that zeolite can also catalyze the filtration for a few species [11, 12, 14]. Other factors that can influence the potential applicability of zeolite are the presence of various-sized zeolite pores (within the submicron range) in membranes. To resolve this issue, crystals of zeolite should be grown in such a manner that flow only occurs through zeolitic pores. But this can enhance the processing steps for synthesizing precise molecular sieves of zeolite.
3 CARBON-BASED MEMBRANES
3 CARBON-BASED MEMBRANES In recent decades, carbon nanotube (CNT) membranes have gained attention for water filtration applications [9, 15, 16]. Research associated with CNT membranes has brought a breakthrough for the understanding of the science related to filtration and its mechanism. However, the use of CNTs is limited because of the complications linked to making their inner hollow cavity in atomic range, which requires a complex synthesis process. On the other hand, a gold nanotube, with an inner diameter of 0.6 nm, has been successfully synthesized . For this purpose, the template-based electrochemical growth technique was employed. Unfortunately, these unique nanotubes have not gained substantial attention because of the complex synthesizing step, along with the issues linked to their reproduction. Graphene, discovered in 2004, has shown outstanding properties in every field it has been tested for. Several studies have shown the properties of pure graphene [18–20]. A pure graphene membrane having zero pores showed a superior permeation flux, mainly because of the tightly packed structure of atoms in the lattice as well as the presence of π-electrons, which repel all the other electrons. Because of its high permeability, graphene can be employed for the synthesis of impermeable capsule shells, gels, and sealed cages. Under normal conditions, using pure graphene films as a molecular sieving agent is still a dare. However, research has been going on to achieve a substantial water flux by using a graphene membrane. Being a two-dimensional (2D) planar structure, graphene has mechanical strength; it requires low pressure to ensure an ultra-fast gas phase and liquidphase filtration.
3.1 CARBON NANOTUBE IN MEMBRANES TECHNOLOGY CNTs are composed of cylindrical-shaped graphite sheets (an allotropic form of carbon) curved up in a roll-like structure with the appearance of a latticework railing . Single-walled carbon nanotubes (SWCNTs) have a cylindrical shape consisting of a single shell of graphene, whereas the multiwalled carbon nanotubes (MWCNTs) consist of more than one layer of graphene sheets. Both classes of CNTs are widely employed directly for desalination purposes [22–24] or indirectly for separating foreign substances that can disturb the desalination process . Using CNTs for desalination is a promising technique because it can require low energy consumption. The flow of water through CNT channels is usually frictionless and allows a specific size range of particles to pass through it. The presence of hollow cylindrical tubes in CNTs with high aspect ratio and the hydrophobic inner tubes improve the flux properties, making it favorable to use for desalination.
3.1.1 Water transport through CNT inner hollow cavity The presence of smooth, hydrophobic inner hollow cavities of CNTs acts in a favor of the natural, continuous flow of water with a very low adsorption rate, as illustrated in Fig. 2. The aligned CNTs in a membrane are of great interest for those fabricating CNT membranes. The pore diameter of the aligned CNTs has a determining effect on the water transport through them. The motion of water molecules through the hollow cavity of CNTs usually follows Fickian motion , which demonstrates the types of molecular motion as, first, a disorderly mass flowing through the cavity whereas, second, the motion of water molecules via a one-directional tube is a single-file mechanism. According to this mechanism, the molecules hinder each other when passing through the tube . The water molecules’ diffusion through the CNTs’ channel is an extremely synchronized movement and can be better elucidated by the ballistic motion of a water chain [26, 28].
CHAPTER 14 CARBON NANOTUBE AND GRAPHENE OXIDE
FIG. 2 Transport of water molecules through hollow CNT structure.
Generally, the water molecules do not follow simple fluids mechanics . The term nanofluidics, instead of simple fluidics, is used to simulate the water movement through the nanotube structure . The water passing through the nanochannels has a slippery nature  in which the water, acting as a nanofluid, slides through the nanochannel with an insignificant change in friction.
3.1.2 Functionalization of CNT To improve the functionality and performance properties of CNT membrane for water purification, they are often subjected to functionalization as a pretreatment process. The pure CNTs often form an agglomerate that considerably drops the water flux, as well as the selectivity of the foreign materials. In general, CNTs are contaminated with metal catalysts, their impurities, and physical heterogeneities . Moreover, CNTs can be crowned into hemispheres that are more like a fullerene curvature during synthesis or the purification step . These crowned CNTs often have opened tips that could easily be oxidized into the desired functional groups that can be used as traps for attracting selective particles. Additionally, the functionalization can be both positive, like NH3 + , or negative, like dCOOd, and sulfonic acids, and, in some cases, hydrophobic, like the aromatic rings on the surface of CNTs [33, 34]. In this way, CNT membranes could be made selective for specific applications, along with an increased flux of water through cylindrical nanoholes, as shown in Fig. 2. The performance properties of functionalized membranes have been shown to have better permselectivity, thermal and chemical stability, increased mechanical strength, fouling resistivity, and self-cleaning functions . The point-end functionalized CNT membrane can have selective groups at the nanotubes’ ends or at the interior core. Both cases have shown enhanced water flux and selectivity of pollutants . The numerous nanoparticles, including Ag, Au, Pt, Cu, TiO2, polymers, and biomolecules, can also be decked on the CNT’s surface to broadened the application for water purification .
3 CARBON-BASED MEMBRANES
3.1.3 Atomic structure and morphology of CNTs CNTs can be imagined as a plane of graphite rolled to form a cylindrical tube, which is distinct from the diamond structure, where a three-dimensional (3D) cubic crystal structure is formed, with each carbon atom having its four nearest neighbors arranged in a tetrahedron. Graphite is designed as a plane sheet of carbon atoms arranged hexagonally. In such cases, the individual carbon atoms have three nearby atoms. Then, the sheet of graphite is rolled to form carbon nanotubes. The characteristics of CNTs are governed by the atomic array (i.e., how the sheet is rolled), the length and the diameter of the nanotube, and the surface morphology.
Nanotube structure The nanotube’s atomic structure is usually portrayed by helicity or the tube chirality. The tube chirality ! is described by chiral angle θ and chiral vector C h. As illustrated in Fig. 3, we can visualize cutting the sheet of graphite along the red line and then rolling the tube so that the tip of the chiral vector dashes is the tail. This is why it also termed a rolled-up vector, commonly represented as Eq. (1): !
C h ¼na1 + ma2 ,
Chiral vector Ch Chiral angle q na1
FIG. 3 Schematic display of graphite sheet rolled to form a nanotube.
CHAPTER 14 CARBON NANOTUBE AND GRAPHENE OXIDE
FIG. 4 Representation of armchair and zigzag structure of carbon nanotubes. !
where n and m represent the number of steps present along the zigzag carbon bonds and a1 and a2 are the unit vectors illustrated in Fig. 3. The amount of twist in the nanotube is determined by the chiral angle. The distinction between zigzag and armchair nanotube structures is described in Fig. 4. The chirality of nanotube structure has a substantial effect on material characteristics. Predominantly, the chirality of tube structure has a strong influence on the electric properties of CNTs. The graphite is considered semimetallic in nature, whereas the CNT can be a semiconductor or metallic in nature depending on to tube’s chirality . The influence of chirality on mechanical properties has been studied. Yakobson et al. [39, 40] studied the instability of nanotubes beyond linear response. The studies showed that CNTs are noteworthy, robust in sustaining harsh strain with no marks of plasticity or brittleness.
3.1.4 Properties of CNT membranes Mechanical properties CNTs are the strongest and hardest materials ever discovered with respect to their tensile strength and elastic modulus, respectively. Such strength arises from the sp2 covalent bond that forms between the carbon atoms, that is, less in the presence of disordered arrangements and defects in the sidewalls of nanotubes. The young modulus of SWCNTs is determined by the chirality and diameter of the nanotube. An experimental study has shown that in the case of MWCNTs, only the outer shell supports stress when nanotubes are incorporated into the matrix phase, whereas in SWCNTs, a prominent decline in the individual modulus has been observed because of poor intertube cohesion . The tensile strength of CNTs can be 50 times greater than steel. These characteristics collectively give the small mass carbon atoms their remarkable potential in various fields, such as aerospace, as first proposed by Arthur C. Clarke. CNTs also have extraordinary electronic properties. It is noteworthy that CNTs can
3 CARBON-BASED MEMBRANES
be metal or semiconductors depending on their chirality. They have higher conductivities that make their possible use in electronic devices, particularly nanobased ones. Still, such useful device nanotubes require thousands be prepared in a specific arranged pattern. To do this, a controlled synthesis step is needed. CNTs are being employed in numerous fields, including the creation of the flat-panel displays of scanning probe microscopes and sensing devices. The remarkable properties of CNTs will indisputably lead to many uses for it [42–46].
Electrical properties CNTs have remarkable electrical properties. A single graphite sheet is semimetal, as it has characteristics between metals and semiconductors. When the graphite planar sheet is twisted to form a nanotube, not only do the carbon atom have to line up around the perimeter of the nanotube, but the quantum mechanical wave functions of the electrons should also be matched. According to theoretical studies, the metallic nanotube can have an electrical current density 1000 times greater than most of the metals such as copper . The macroscopic structures of a singular nanotube can be elucidated by several electrical properties, such as capacitance, resistance, and inductance, that are due to intrinsic structure of nanotube and its interaction with other things. The transport of electricity inside the hollow cylindrical nanotube can be affected by defects, scattering phenomena and through lattice vibrations that primarily lead to resistance analogous to bulk material. However, the one-dimensional (1D) character of CNTs, along with their solid covalent bonding, considerably affects these processes. In 1D material, the scattering phenomena by small angles is generally not allowed as there is only frontward and backward motion of carrier occur. Significantly, the 1D character of CNTs cause the new type of quantized resistance linked to its interaction with 3D macroscopic materials, such as metallic electrodes. In addition, with quantized resistance, several new types of interaction resistance, such as Schottky barriers at metal-semiconducting nanotube interfaces, and parasitic resistance are simply due to bad contacts. The intrinsic structures of CNTs lead to capacitance mainly linked to the density of states and its independence from electrostatics. Last, CNTs have inductance that resists any change in the current flowing through the nanotubes. Conventionally, inductance depends on the diameter of the nanotube, its geometrical structure, and the magnetic permeability of the media. CNTs often behave as transmission lines, owing to their inductance in response to the alternating current signal [42, 44].
Thermal properties It is anticipated that all nanotubes have a high thermal conductivity, particularly along the axis, demonstrating the characteristics termed “ballistic conduction.” It is expected that nanotubes will transmit up to 6000 W m1 K1 at ambient temperature in comparison to copper, which only transmits 385 W m1 K1. The thermal stability of CNTs is up to 2800°C in vacuum and 750°C in air media. In traditional graphite fibers, thermal expansion is strongly anisotropic; in contrast, CNT thermal expansion is mainly isotropic. Such a property can be beneficial for carbon-carbon composites. It is predicted that CNTs with few defects will show low thermal expansion coefficients [46, 47].
Chemical properties The curved graphene sheet showed a high thermal stability as compared to the planar graphite sheet. The curvature allows the mixing of σ- and π-orbital, leading to hybridization among the orbitals. As the diameter of SWCNTs gets smaller, the degree of hybridization increases as the reactivity of CNTs is directly dependent on the mismatched π-orbital because of the increased curve. For that reason,
CHAPTER 14 CARBON NANOTUBE AND GRAPHENE OXIDE
a difference must be prepared between the sidewall and the tip-end caps of a nanotube. Also the smalldiameter nanotube shows high reactivity. The side walls or tip-end caps can be covalently modified; for example, the solubility of CNTs in numerous solvents can be controlled in such a way, whereas achieving the covalent bond attachment to any molecular species to fully sp2-bonded carbon atoms on sidewalls of nanotubes is quite difficult. Hence, CNTs can be considered chemically inert in nature .
Optical properties In the case of SWCNTs, the optical properties of nanotubes are connected to their quasi-1D nature. Several studies theoretically conducted have demonstrated that the optical nature of chiral CNTs diminishes as the size of nanotubes increases to a certain limit. Consequently, it is likely that other physical characteristics are also affected by these factors. The applicability of the optical activity of CNTs allows it to be used in optical devices .
3.1.5 Application of CNTs in desalination Having clean, safe water is one of the basic human rights. Unfortunately, that right has been deteriorating with population increases, urbanization, and climate change. These factors not only have stalled development of humans but have also created an imbalance in nature cycle [50, 51]. With the advancement in nanotechnology, many impressive nanomaterials, including carbon nanotubes , nano-zinc particles , electrospun nanofibers , and numerous other nanoparticles, have been employed for purifying water, and in particular, CNTs have shown remarkable achievements in purifying wastewater . The current desalination process mostly depends on polymeric reverse-osmosis membranes for separating out the dissolved salts and fine solids . For this process, high pressure is required, which means that high energy consumption is needed to drive the desalination plant. There also exists a high trade-off between the high selectivity and high permeation flux in the membrane design process. In the last few decades, theoretically calculated  and experimental  studies have been demonstrated that water transport through nanotubes is several orders of magnitude higher than that through porous materials of comparable size, owing to the high velocity attributed to the smooth, hydrophobic nature of inner cylindrical walls of CNTs. Ordered hydrogen bonds are formed at the interface of water and CNTs that initiate a vapor phase barrier between the nonpolar CNT wall and water molecular chain, causing the frictionless movement of water molecules inside the hollow cylindrical tube. The aligned CNT structural membranes are responsible for the highest permeation flux. Recently, 2-nm aligned membranes have been developed employing the chemical vapor deposition process, followed by a laser-etching process to uncap the nanotubes . The permeation of water molecules through these membranes are of several orders of magnitude higher than the commercially available polycarbonate membranes despite having a smaller pore size. To fully use the hollow structure of CNTs, a vertically aligned high-density membrane was synthesized by Yu et al. . The CNT arrangement was made using a chemical vapor deposition process, and then CNT was immersed in an organic solvent, such as n-hexane; then formed layers were dried at room temperature. The evaporation process decreased the layer size up to 5% of its original size, which led to an increased density and a crowded, vertically arranged CNT structure. The tip of a CNT membrane can be functionalized by achieving ion exclusion. Gong et al.  fabricated the ion-selective, controlled nanopores based on SWCNTs with arranged carbonyl oxygen group atoms inside the nanotube. The varying pattern of carbonyl oxygen atoms determined the
3 CARBON-BASED MEMBRANES
hydration structure of Na+ and K+ within the hollow structure, which led to tunable ion selectivity. In their work, Majumder et al.  functionalized the tips of the CNT structure via an electrochemical grating process using diazonium salts, and they suggest that the separation efficiency of CNTs can be altered by changing voltage. Fornasiero and coworkers  introduced a negatively charged functional group via a plasma treatment process that caused an ion rejection up to 98% through an aligned CNT membrane; also, the ion-exclusion process was dominated by the charge-exclusion process. However, in a high ion-concentrated environment such as the sea or brackish water, the separation ability of the charge-exclusion process can decrease considerably. Until now, the smallest diameter achieved for CNTs is 0.3 nm , which is roughly equal to the radius of hydrated sodium ions, which ranges from 0.178 to 0.358 nm, depending on environmental conditions [63, 64] Consequently, fabricating defect-free CNT membranes that have subnanometer pore size can shine a light on future desalination technologies.
3.1.6 Potentiality of CNT membranes CNT membranes consist of nanopores that are ideal for rejecting micropollutants and ions mostly in the liquid phase. The presence of hydrophobic inner walls in cylindrical nanotubes allows the flow of water with almost zero friction, negating the need of any external force to push the water molecules through the hollow cylindrical pore. CNT membranes have shown less foulant attachment between of cytotoxic effects that kill or eradicate pathogens, thus ultimately increasing the membranes’ lives. The selective synthesis or functionalization of CNTs allows the rejection of selective pollutants from water [34, 37]. Last, CNTs can be modified for reuse with less complexity, high durability, and environmentally friendly, devoid of any complicated chemical alteration.
3.2 GRAPHENE OXIDE The graphene-based materials have been widely studied for numerous thin-film and membrane application as they have unique 2D structure, are only one atom wide, and have remarkable mechanical strength and excellent flexibility [65–67]. Graphene oxide (GO), a derivative of graphene material, has gained an immense attraction for the development of ultra-thin and high-permselective membranes. Because they have a high area-to-thickness ratio and great number of functional groups, GO fragments can be loaded on each other such that they arrange to form thin film or membrane [66, 68]. Graphene oxide (GO) has become one of the excellent materials for membrane fabrication. In 2012, a study demonstrated that a GO membrane allows unrestricted flow of water through it but hinders everything else in vapor form . However, this study did not rule out the joint propagation of organic molecules present in water passing through the GO membrane. The ease of fabricating the thin GO layers to form the membrane act in favor of their practical use. Generally, graphene does not allow anything to pass through it. However, graphene oxide (GO) has constantly shown superior membrane properties and provides a great potential for commercial use.
3.2.1 Graphene oxide membrane Graphene-based functional membranes have gained recent attention as outstanding candidates for filtration and separation processes because of to their porous microstructure [70, 71]. Unimpeded permeation flux of water through the submicrometer-thick GO membranes was compared with impermeable membranes for a performance study for liquids, gases, and vapors, such as helium. The high
CHAPTER 14 CARBON NANOTUBE AND GRAPHENE OXIDE
permeability is attributed both to the capillary-driven force and low friction flow that are present between the 2D channels of pure graphene . As the derivative of graphene, the advancements of GO and reduced graphene forms have moved toward the use or water purification purpose [72–75]. Distinct form the nanosheets of graphene that have nanopores, the selective separation property is mainly due to the presence of numerous nanochannels inside the assembled membranes that compose an interlayer gallery, lengthened paths, and the functional groups present on the surface . Because of the abundance of oxygen-containing functional groups inside the GO nanosheets, it is facile to arrange them into the laminar-structure membrane through spray coating, spin or dip coating, vacuum filtration, or layer-by-layer assembly techniques .
3.2.2 Preparation of GO membrane GO can be generally prepared by an amended Hummers method, where graphite flakes are used as starting material [76, 77]. In the synthesis process, graphite flakes are first subjected to oxidization by employing strong oxidizing agents, such as NaNO3, KMnO4, and concentrated sulfuric acid. The single-layer GO sheets are then exfoliated by long, continuous stirring or are ultrasonicated . Compared with graphene surface, these chemically treated GO flakes have numerous functional groups on their edges and surface, for example, carboxyl and hydroxyl groups . The presence of the hydroxyl groups on the GO flakes allows them to dissolve in water or any other polar solvents, thus reducing the cost of forming graphene-oxide-based materials, such as GO thin films [67, 79, 80]. The initial crystal size of the graphite flakes and the purification stage govern the diameter of GO flakes, which differ from several hundred nanometers to micrometers. Through a self-assembly process, GO flakes are arranged on top of each other, forming a continuous laminar-structure membrane. Between the GO flakes exists a hydrogen bonding responsible for the higher mechanical strength . Although a freestanding thick GO membrane can be synthesized , conventionally an ultra-thin membrane is maintained on a porous substrate to enhance the mechanical strength and ease of handling. The porous substrate can be either polymeric or inorganic material, either in the form of a hollow fibrous structure or a flat sheet [72, 81, 82]. There are numerous processes to synthesize GO membranes; the simplest is by vacuum filtration. In this process, the GO suspension is filtered onto a substrate so that the width of the membrane can be skillfully controlled by the volume of GO filtered. Several studies have suggested that the during the filtration step, the driving force can alter the arrangement of GO sheets in the film . Moreover, in addition to pressure-controlled processes, some fabrication methods employ the surface tension of the liquid for the self-assembly technique of GO sheets. Another method is the evaporation method, which involves heating the GO suspension up to 80°C . The rapid evaporation occurs at the liquid-air interface, ultimately causing to GO sheets to self-assemble and thus their arrangement into a thin film or membrane of GO. Other methods include dip coating, drop coating, and spray coating. In these methods, a suspension of GO is dispersed onto supporting material, and after drying, a GO membrane formed [69, 81].
3.2.3 GO membrane filtration mechanism A study has demonstrated that a GO membrane with submicrometer thickness can absolutely hinder the flow of liquid and gas molecules, only allowing the permeation of water vapors . This might be due to the presence of an empty interspace between the nonoxidized GO sheets that allows the transport of water vapors through low-friction channels. In another study, the coefficient of water diffusion in these
3 CARBON-BASED MEMBRANES
FIG. 5 Schematic display of proposed separation mechanism (A) size exclusion, (B) Donnan exclusion, and (C) adsorption phenomena.
GO nanochannels was illustrated to have 4–5 orders of magnitude, which is generally higher than most of the polymeric membranes. Thus, GO membranes can also be employed for ultra-fast liquid water permeation . From these research findings, a tremendous amount of research on GO membranes for filtration purpose has been done. Fig. 5 demonstrates all the possible filtration mechanisms of GO membranes in the filtration application. Through the size-exclusion process, the bulky organic molecules could be filtered because of the presence of nanochannels in GO membranes. According to one study, the spacing between GO sheets can be manipulated to increase or decrease the size of nanochannels for the precise separation of ionic species or bulky molecules . Hence, for desalination, water purification, and other pharmaceutical filtration, one can fabricate the specific GO membrane with specific interlayer spacing between GO sheets or by incorporating the nanofiller or nanoparticles with a desired size for desired applications. Moreover, GO membranes can be subjected to reduction to eliminate the hydrophilic functional groups present on the edges and surface of GO that lead to a decrease in d-spacing. The reduced GO can be prepared either by chemical reduction or thermal annealing in order to remove the oxygen-based functional groups . The simplest and most effective method for reducing GO by eliminating oxygen-containing functional groups, particularly OH groups, is thermal annealing . A rise in temperature assists the thermal deoxygenation of GO. However, in this process, high energy consumption is required, and the degree of oxidation is also difficult to control. On contrary, the chemical reduction of GO required a low temperature range by the addition of reducing agents, such as metal hydrides, hydrazine, and hydroiodic acid . Such reducing agents target different functional groups, thus allowing control over the whole reduction process. The reduced GO provides the channels at the angstrom level without conceding the permeability of water, which is mainly ideal for ionic-level filtration . Also, the prepared GO membranes can be reduced by chemical reduction, providing that the reduced nanochannels have an increased hydrophobic character. Besides the size-exclusion effect,
CHAPTER 14 CARBON NANOTUBE AND GRAPHENE OXIDE
the material could be separated by Donnan exclusion process [89, 90]. The GO membrane is negatively charged because of the removal of a proton from the carboxyl group present on the edge or tip of the GO sheet. This causes the pure GO membrane to reject the negatively charged organic species or divalent ions [20, 91]. Nevertheless, the charge on GO membrane can be altered . The remarkable rejection can be achieved by the strong adsorption of small ionic species via various interactions with varying regions on GO sheets . This was attributed to the fact that the transition metal cations can form a coordinate interaction with any oxygen-containing functional groups, leading to a complete blockage by GO membrane . In the same way, the permeability of alkaline earth metals and alkali are also predominantly lessened because of the interaction with the sp2 cluster of GO sheets via cation-π interactions .
3.2.4 Microstructures of GO membranes The microstructure of the GO membrane includes the stacking of GO sheets and the defects present in the membrane that can be influenced by the synthesizing step, which ultimately affects the performance properties of the GO membrane. A study has revealed that a GO membrane fabricated by the drop- or spin-casting method has a denser packed structure and showed a high selectivity for CO2 . Another study revealed that among GO membranes prepared by three different process—vacuum-assisted filtration, pressure-assisted filtration, and evaporation —the membrane prepared by pressure-assisted filtration process illustrated superior performance properties in butanol dehydration, predominantly because of the arranged laminar structure. The surface roughness and hydrophilicity of GO membranes are the main parameters that can influence the membrane microstructures. The magnitude of the GO sheets can be influenced the microstructure and thus performance properties of GO membranes in terms of permeability and selectivity . The use of nanosized GO sheets for fabricating membranes showed fewer crumples and folds on the surface when compared to membranes prepared by the use of micron-size GO sheets, even though the interlayer space distance remained constant in both cases. However, XRD results showed a broad peak range in the case of nanosized GO sheets. Moreover, the ions’ flow through nanosized GO membrane was also enhanced, mainly because of the less densely packed laminar structure. In a study, GO paper was prepared from large GO sheets showed a more compact structure with ordered microstructures and less structural defects than those fabricated from small GO sheets. Also they showed a superior mechanical strength . The influence of the size of GO sheet used in membranes was studied regarding the evaporation process . The large and bulky micron-sized GO sheet was inclined to move toward the water surface, causing the form of continuous membrane formation after the drying step, while nanosized GO sheets tended to disperse in the water phase, causing a “coffee-ring-stain” type of pattern after drying. This might be due to the increase in surface charge density as a consequence of enhanced edge-to-area ratio.
3.2.5 Modifications, challenges, and prospects Several alterations have been done to improve the performance properties of GO membranes. Several approaches, including the pore formation of GO sheet and the microstructural path formation, have been tested for forming additional transport channels in pure GO membranes that can ultimately reduce the water transport pathway and hence increase the permeability of water, as shown in Fig. 6 [99, 100]. However, the selectivity of the membrane may be compromised, dropping the filtration property of the
3 CARBON-BASED MEMBRANES
FIG. 6 Water flow through pure graphene oxide and pores generated graphene oxide.
GO membrane. Several studies have been done on cross-linking GO sheets or the decoration of GO sheets with polymeric materials or nanoparticles [91, 101, 102]. The GO-flake interlayer can be modified for selective separation purposes. The increased interaction between the sheets or the flakes of GO ensures the high stability of the membrane. Even though the GO membrane has hydrophilic character, several studies have further improved the hydrophilicity, showing much better results for butanol dehydration . The reduced form of GO has also shown high performance properties in terms of permeability and selectivity in the forward-osmosis and nanofiltration processes [104, 105]. Regardless of the all the remarkable discoveries for the research of GO membranes, some challenges for the commercial application of GO membranes exist. One of the major issues is the stability of GO membranes. Recent research has depicted the implication of ceramic material, as a substrate, releasing various multivalent ions that allow the cross-linking of GO sheets, ultimately improving the stability of membrane in the aqueous phase. On the other hand, polymeric material, when used as a substrate, showed instability in the aqueous phase . Moreover, GO membranes have also shown instability in the air medium as they reduce in size after the drying process. The reduction issue can be solved by storing the membranes in the water phase to avoid excessive drying  or by employing the upper sacrificial coating during membrane preparation . Further work is required to solve the stability issue of GO membranes, mainly where the membrane width is just at the submicron level. In addition, there are also some limitations on how to characterize GO membranes in several studies. Their uses beyond fluid filtration can also be explored further.
3.2.6 Comparison of CNTs and graphene oxide-based membranes with other conventional membranes Conventional RO and NF membranes have shown dense porous structures with good separation properties that can be employed because of their easy fabrication and comparatively low cost. Also, these membranes require that pressure be applied to force the molecules of water to pass through them. On the other hand, MF and UF technologies require less energy consumption but separate out only the suspended solid particles [28, 108], whereas polymer-based membranes have some restrictions, such
CHAPTER 14 CARBON NANOTUBE AND GRAPHENE OXIDE
as poor resistance toward chemicals and high temperature, membrane fouling, and aging under extreme conditions, mostly in organic solvents . Carbon-based materials, such as CNTs and graphene, or its derivatives GO, have been widely studied because of their easy availability, high mechanical strength, and chemical, as well as thermal, stability [110, 111]. GO can be economically prepared from the pure graphitic flakes via the modified Hummer’s method . It consist of single layer of atomic structure having both sp2 CC and sp3 CO bonds and numerous oxygen-containing groups, including hydroxyl, carbonyl, and epoxy groups, situated at the basal region and on edges of graphite sheet [111a]. The lateral dimension of GO sheet ranges from nanometers to a few micrometers [111b]. Owing to their high aspect ratio, GO sheets can be arranged on each other to form a thin laminate membrane  with excellent separation performance properties for numerous applications, such as gas separation , membrane filtration , and pervaporation . Additionally, mixed matrix membranes composed of functionalized GO sheets can increase the separation efficiency and overall membrane performance [111c]. Owing to the ultra-fast property of water flow through the carbon nanochannels, GO membranes have great potential in the field of desalination. The hydrophobic hollow inner cylinders of CNTs allow the frictionless movement of polar water molecules. The presence of nanoscale pore sizes rejects the movement of salts and retains the ions. The choice of membrane type is totally determined by its functionality, energy consumption, robustness, permeability of water, antifouling capability, and selectivity toward contamination. CNT-based membranes have predominantly shown excellent permeation of water molecules, as well as selectivity of salts, thus making them attractive for desalination process [28, 112, 113]. The aligned CNT membranes have been proved to have excellent permeability compared to conventional polymeric RO membranes. Cohen and his coworkers  have employed CNT membranes as substitutes for RO membranes to separate salt from wastewater. The altered membranes have shown excellent separation compared to RO membrane ; also, they overpower the limitations faced with conventional membranes when employed for water purification techniques. The salt-selectivity capability of CNT-based membranes have shown almost similar performance properties to that of commercial NF membranes . Also, CNT membranes with pore sizes smaller than 2 nm were synthesized ; they not only showed an increase in the selectivity of ions but also demonstrated better performance than conventional polycarbonate membranes. Today, research is mainly focus on achieving the pore size smaller than 1 nm that will retain almost all solute particles. By modifying the surface properties of CNTs, it is possible to separate out smaller ionic solutes with high selectivity and greater affinity . Research has been conducted showing that modifying the surface charge of the CNT structure can cause the removal of Na+. The 100% removal efficiency of K3Fe(CN)6 has been studied employing carboxyl functional CNT arrays. Such an arrangement forms an electrostatic repulsion at the tips of the CNTs, thus successfully retaining the salt ions. Chan et al.  formed the simulation, as well as synthetically formed a CNT membrane with a diameter of 1.5 nm, having two zwitterions at the end of tips, that provide 100% rejection, while 20% rejection was achieved in the case of five carboxyl groups present at the tip end of CNTs. The combined effect may be due to the steric hindrance and electrostatic cloud present at the nanotubes’ ends. Ratto and his coworkers  have patented their research showing that CNT membranes shown an ion-rejection capability higher than 99%, demonstrating a remarkable achievement in the field of desalination.
3.2.7 Conclusion and future perspective Pressure-driven membranes are widely used for wastewater purification and in pharmaceutical industry. The exceptional physical and mechanical characteristics shown by carbon-based materials, carbon nanotubes, and graphene oxide, combined with their low density and high area-to-volume ratio, make them suitable candidates for membrane fabrication. The ideal ultra-fast membrane is predicted to have an extremely low thickness to ensure high permeability and mechanical strength for withstanding the applied pressure. Today, there is alarming situation requiring the development of a membrane with the prospect of potential application in environmental research. Such ideal membranes should also exhibit the high selectivity and remarkable permeability. Even though numerous polymeric membranes have been developed for specific purposes, they have shown low permeance. Some shortcomings of using such polymeric membranes for energy, as well as environmental, purposes are their poor temperature resistivity and chemical stability in presence of acid, bases, or organic solvents [118, 119]. All the previously mentioned problems linked to polymeric membranes have led to the development of substitute membranes. Owing to their superior mechanical strength, chemical stability, accessibility of functional groups, and eco-friendly nature, carbon-based materials are being extensively researched for membrane purpose. Primarily, CNTs are considered as a remarkable contender for membrane fabrication mainly because of their 1D hollow cylindrical structure, along with their superior mechanical property. Nevertheless, the commercial application of these vertically aligned CNTs for membrane fabrication is quite challenging. Consequently, using CNTs membranes at the commercial scale remains theoretical [113, 120]. Then, the amorphous carbon structure, such as that of diamonds, has been employed for membrane fabrication because of to their harness and chemically inert behavior [121, 122]. However, their real-life use is also very restricted, owing to their high energy utilization and the size of equipment needed . We consider GO to be the material of interest for membrane use. Recent research on the stability on GO in the aqueous phase has paved the way for its future use . The numerous studies reporting on GO membranes [69, 124], along with GO being used as a layered material , will maintain the versatile future of the GO. Definitely, there are some advantages and disadvantages regarding the experimental results and the proposed transport mechanism. Nonetheless, these can be undoubtedly understood in the near future through ongoing continuous efforts. Compared with other membrane materials, GO membranes foremost have a superiority owing to the simplicity of their fabrication method, which provides a uniform pore-size distribution throughout the membrane. Moreover, the GO membrane can be altered according to the needs for real-time application. Also, the thin membrane, with its high permselectivity, is also linked to issues such as reproducibility, durability, and scalability. To the contrary, the multilayer membranes have prospects for real-life applications because their thickness can be controlled, but they also have some restrictions, such as the thermal stability of GO membrane .
REFERENCES  R.K. Joshi, S. Alwarappan, M. Yoshimura, V. Sahajwalla, Y. Nishina, Graphene oxide: the new membrane material, Appl. Mater. Today 1 (1) (2015) 1–12, https://doi.org/10.1016/j.apmt.2015.06.002.  D.F. Sanders, Z.P. Smith, R. Guo, L.M. Robeson, J.E. McGrath, D.R. Paul, B.D. Freeman, Energy-efficient polymeric gas separation membranes for a sustainable future: a review, Polymer 54 (18) (2013) 4729–4761, https://doi.org/10.1016/j.polymer.2013.05.075.
CHAPTER 14 CARBON NANOTUBE AND GRAPHENE OXIDE
 P. Shao, R.Y.M. Huang, Polymeric membrane pervaporation, J. Membr. Sci. 287 (2) (2007) 162–179, https://doi.org/10.1016/j.memsci.2006.10.043.  M. Ulbricht, Advanced functional polymer membranes, Polymer 47 (7) (2006) 2217–2262, https://doi.org/ 10.1016/j.polymer.2006.01.084.  C. Zhao, S. Nie, M. Tang, S. Sun, Polymeric pH-sensitive membranes—a review, Prog. Polym. Sci. 36 (11) (2011) 1499–1520, https://doi.org/10.1016/j.progpolymsci.2011.05.004.  X. Chen, S.Y.E. Yeo, J.Y.I. Woo, Y.E. Zhou, L. Hong, Lanthanum-doped kaolinite for hierarchical bi-modal porous inorganic membrane, J. Eur. Ceram. Soc. 37 (10) (2017) 3443–3451, https://doi.org/ 10.1016/j.jeurceramsoc.2017.04.009.  L. Cot, A. Ayral, J. Durand, C. Guizard, N. Hovnanian, A. Julbe, A. Larbot, Inorganic membranes and solid state sciences, Solid State Sci. 2 (3) (2000) 313–334, https://doi.org/10.1016/S1293-2558(00) 00141-2.  T.L. Ward, T. Dao, Model of hydrogen permeation behavior in palladium membranes, J. Membr. Sci. 153 (2) (1999) 211–231, https://doi.org/10.1016/S0376-7388(98)00256-7.  M. Wasim, A. Sabir, M. Shafiq, A. Islam, T. Jamil, Preparation and characterization of composite membrane via layer by layer assembly for desalination, Appl. Surf. Sci. 396 (2017) 259–268, https://doi.org/ 10.1016/j.apsusc.2016.10.098.  J. Caro, M. Noack, Zeolite membranes – recent developments and progress, Microporous Mesoporous Mater. 115 (3) (2008) 215–233, https://doi.org/10.1016/j.micromeso.2008.03.008.  L. Li, J. Dong, T.M. Nenoff, R. Lee, Desalination by reverse osmosis using MFI zeolite membranes, J. Membr. Sci. 243 (1) (2004) 401–404, https://doi.org/10.1016/j.memsci.2004.06.045.  L. Li, N. Liu, B. McPherson, R. Lee, Influence of counter ions on the reverse osmosis through MFI zeolite membranes: implications for produced water desalination, Desalination 228 (1) (2008) 217–225, https://doi. org/10.1016/j.desal.2007.10.010.  E.E. McLeary, J.C. Jansen, F. Kapteijn, Zeolite based films, membranes and membrane reactors: progress and prospects, Microporous Mesoporous Mater. 90 (1) (2006) 198–220, https://doi.org/10.1016/j. micromeso.2005.10.050.  M. Severance, B. Wang, K. Ramasubramanian, L. Zhao, U.S. Winston Ho, P.K. Dutta, Rapid crystallization of Faujasitic zeolites, Langmuir 30 (2014) 6929–6937.  W. Falath, A. Sabir, K.I. Jacob, Highly improved reverse osmosis performance of novel PVA/DGEBA cross-linked membranes by incorporation of Pluronic F-127 and MWCNTs for water desalination, Desalination 397 (2016) 53–66, https://doi.org/10.1016/j.desal.2016.06.019.  A. Sabir, M. Shafiq, A. Islam, A. Sarwar, M.R. Dilshad, A. Shafeeq, T. Jamil, Fabrication of tethered carbon nanotubes in cellulose acetate/polyethylene glycol-400 composite membranes for reverse osmosis, Carbohydr. Polym. 132 (2015) 589–597, https://doi.org/10.1016/j.carbpol.2015.06.035.  K.B. Jirage, J.C. Hulteen, C.R. Martin, Nanotuble-based molecular-filtration membranes, Science 278 (1997) 655–658.  M.S.H. Boutilier, C. Sun, S.C. O’Hern, A. Harold, N.G. Hadjiconstantinou, R. Karnik, Implications of permeations through intrinsic defects in graphene on the design of defect-tolerant membranes for gas separation, ACS Nano 8 (1) (2014) 841–849.  S.C. O’Hern, M. Boutilier, J.C. Idrobo, Y. Song, J. Kong, T. Laoui, M. Atieh, R. Karnik, Selective ionic transport through tunable sub-nanometer pores in single-layer graphene membranes, Nano Lett. 14 (3) (2014) 1234–1241.  Y. Han, Z. Xu, C. Gao, Ultrathin graphene nanofiltration membrane for waterpurification, Adv. Funct. Mater. 23 (29) (2013) 3693–3700.  E.T. Thostenson, Z. Ren, T.-W. Chou, Advances in the science and technology of carbon nanotubes and their composites: a review, Compos. Sci. Technol. 61 (13) (2001) 1899–1912, https://doi.org/10.1016/ S0266-3538(01)00094-X.
 K. Dai, L. Shi, D. Zhang, J. Fang, NaCl adsorption in multi-walled carbon nanotube/active carbon combination electrode, Chem. Eng. Sci. 61 (2) (2006) 428–433, https://doi.org/10.1016/j. ces.2005.07.030.  H. Li, L. Zou, Ion-exchange membrane capacitive deionization: a new strategy for brackish water desalination, Desalination 275 (1) (2011) 62–66, https://doi.org/10.1016/j.desal.2011.02.027.  A.T. Nasrabadi, M. Foroutan, Ion-separation and water-purification using single-walled carbon nanotube electrodes, Desalination 277 (1) (2011) 236–243, https://doi.org/10.1016/j.desal.2011.04.028.  L. Joseph, J. Heo, Y.-G. Park, J.R.V. Flora, Y. Yoon, Adsorption of bisphenol A and 17α-ethinyl estradiol on single walled carbon nanotubes from seawater and brackish water, Desalination 281 (2011) 68–74, https:// doi.org/10.1016/j.desal.2011.07.044.  A. Striolo, The mechanism of water diffusion in narrow carbon nanotubes, Nano Lett. 6 (4) (2006) 633–639.  D.G. Lcvitt, Dynamics of a single-file pore: non-Fickian behavior, Phys. Rev. A 8 (6) (1973) 3050–3054.  C.H. Ahn, Y. Baek, C. Lee, S.O. Kim, S. Kim, S. Lee, … J. Yoon, Carbon nanotube-based membranes: fabrication and application to desalination, J. Ind. Eng. Chem. 18 (5) (2012) 1551–1559, https://doi.org/ 10.1016/j.jiec.2012.04.005.  J.A. Thomas, A.J.H. McGaughey, Reassessing fast water transport through carbon nanotubes, Nano Lett. 8 (9) (2008) 2788–2793.  J.K. Holt, Carbon nanotubes and nanofluidic transport, Adv. Mater. 21 (5) (2009) 3542–3550.  M.S. Mauter, M. Elimelech, Environmental applications of carbon-based nanomaterials, Environ. Sci. Technol. 42 (16) (2008) 5843–5859.  J. Li, H.T. Ng, A. Cassell, W. Fan, H. Chen, Y. Qi, J. Koehne, J. Han, M. Meyyappan, Carbon nanotube nanoelectrode array for ultrasensitive DNA detection, Nano Lett. 3 (5) (2003) 597–602.  P.S. Goh, A.F. Ismail, B.C. Ng, Carbon nanotubes for desalination: performance evaluation and current hurdles, Desalination 308 (2013) 2–14, https://doi.org/10.1016/j.desal.2012.07.040.  S. Kar, R.C. Bindal, P.K. Tewari, Carbon nanotube membranes for desalination and water purification: challenges and opportunities, Nano Today 7 (5) (2012) 385–389, https://doi.org/10.1016/j.nantod. 2012.09.002.  X. Qu, P.J.J. Alvarez, Q. Li, Applications of nanotechnology in water and wastewater treatment, Water Res. 47 (12) (2013) 3931–3946, https://doi.org/10.1016/j.watres.2012.09.058.  M. Majumder, B. Corry, Anomalous decline of water transport in covalently modified carbon nanotube membranes, Chem. Commun. 47 (27) (2011) 7683–7685.  E. Van Hooijdonk, C. Bittencourt, R. Snyders, J.F. Colomer, Functionalization of vertically aligned carbon nanotubes, Beilstein Int. J. Nanotechnol. 4 (1) (2013) 129–152.  M.S. Dresselhaus, G. Dresselhaus, P.C. Eklund, Electronic Structure Science of Fullerenes and Carbon Nanotubes, Academic Press, San Diego, 1996, pp. 413–463 (Chapter 12).  B.I. Yakobson, C.J. Brabec, J. Bernholc, Nanomechanics of carbon tubes: instabilities beyond linear range, Phys. Rev. Lett. 76 (14) (1996) 2511–2514.  B.I. Yakobson, G. Samsonidze, G.G. Samsonidze, Atomistic theory of mechanical relaxation in fullerene nanotubes, Carbon 38 (11) (2000) 1675–1680, https://doi.org/10.1016/S0008-6223(00)00093-2.  P.J.F. Harris, Carbon Nanotubes and Related Structures: New Materials for the 21st Century, Cambridge University Press, Cambridge, 1999.  P.R. Bandaru, Electrical properties and applications of carbon nanotube structures, J. Nanosci. Nanotechnol. 7 (2007) 1–29.  M.B. Nardelli, J.L. Fattebert, D. Orlikowski, C. Roland, Q. Zhao, J. Bernholc, Mechanical properties, defects and electronic behavior of carbon nanotubes, Carbon 38 (11) (2000) 1703–1711, https://doi.org/ 10.1016/S0008-6223(99)00291-2.  H. Dai, A. Javey, E. Pop, D. Mann, Y. Lu, Electrical transport properties and field effect transistors of carbon nanotubes, Nano Lett. (1) (2006) 1.
CHAPTER 14 CARBON NANOTUBE AND GRAPHENE OXIDE
 M. Meo, M. Rossi, Prediction of Young’s modulus of single wall carbon nanotubes by molecular-mechanics based finite element modelling, Compos. Sci. Technol. 66 (11) (2006) 1597–1605, https://doi.org/10.1016/ j.compscitech.2005.11.015.  E. Pop, D. Mann, J. Cao, Q. Wang, K. Goodson, H. Dai, Negative differential conductance and hot phonons in suspended nanotube molecular wires, Phys. Rev. Lett. (15) (2006) 95.  H. Stahl, J. Appenzeller, R. Martel, P. Avouris, B. Lengeler, Intertube coupling in ropes of single-wall carbon nanotubes, Phys. Rev. Lett. 85 (2000) 5186.  V. Lordi, N. Yao, Molecular mechanics of binding in carbon-nanotube-polymer composites, J. Mater. Res. 15 (12) (2000) 2770–2779.  H. Kataura, Y. Kumazawa, Y. Maniwa, I. Umezu, S. Suzuki, Y. Ohtsuka, Y. Achiba, Optical properties of single-wall carbon nanotubes, Synth. Metals 103 (1) (1999) 2555–2558, https://doi.org/10.1016/S03796779(98)00278-1.  A. Sabir, A. Islam, M. Shafiq, A. Shafeeq, M.T.Z. Butt, N.M. Ahmad, … T. Jamil, Novel polymer matrix composite membrane doped with fumed silica particles for reverse osmosis desalination, Desalination 368 (2015) 159–170, https://doi.org/10.1016/j.desal.2014.12.041.  M. Wasim, A. Sabir, M. Shafiq, A. Islam, M. Azam, T. Jamil, Mixed matrix membranes: two step process modified with electrospun (carboxy methylcellulose sodium salt/sepiolite) fibers for nanofiltration, J. Ind. Eng. Chem. 50 (2017) 172–182, https://doi.org/10.1016/j.jiec.2017.02.011.  M. Wasim, S. Sagar, A. Sabir, M. Shafiq, T. Jamil, Decoration of open pore network in polyvinylidene fluoride/MWCNTs with chitosan for the removal of reactive orange 16 dye, Carbohydr. Polym. 174 (2017) 474–483, https://doi.org/10.1016/j.carbpol.2017.06.086.  A. Sabir, W. Falath, K.I. Jacob, M. Shafiq, N. Gull, A. Islam, T. Jamil, Integrally skinned nano-cellular crosslinked asymmetric thin films infused with PEO-PPO-PEO block copolymer/ZnO-NPs for desalination using sea salt, Mater. Chem. Phys. 183 (2016) 595–605, https://doi.org/10.1016/j.matchemphys. 2016.09.022.  A. Sabir, W. Falath, K.I. Jacob, M. Shafiq, M.A. Munawar, A. Islam, T. Jamil, Hyperbranched polyethyleneimine induced polycationic membranes for improved fouling resistance and high RO performance, Eur. Polym. J. 85 (2016) 266–278, https://doi.org/10.1016/j.eurpolymj.2016.10.032.  G. Hummer, J.C. Rasaiah, J.P. Noworyta, Water conduction through the hydrophobic channel of a carbon nanotube, Nature 414 (2001) 188–190.  M. Majumder, N. Chopra, R. Andrews, B.J. Hinds, Nanoscale hydrodynamics-enhanced flow in carbon nanotubes, Nature 438 (44) (2005).  J.K. Holt, H.G. Park, Y. Wang, M. Stadermann, A.B. Artyukhin, C.P. Grigoropoulos, A. Noy, O. Bakajin, Fast mass transport through sub-2-nanometer carbon nanotubes, Science 312 (5776) (2006) 1034–1037.  M. Yu, H.H. Funke, J.L. Falconer, R.D. Noble, High density, vertically aligned carbon nanotube membranes, Nano Lett. 9 (1) (2009) 225–229.  X. Gong, J. Li, X. Ke, J. Wang, H. Yang, A controllable molecular sieve for Na+ and K + ions, J. Am. Chem. Soc. 132 (6) (2010) 1873–1877.  M. Majumder, X. Zhan, R. Andrews, B.J. Hinds, Voltage gated carbon nanotube membranes, Langmuir 23 (16) (2007) 8624–8631.  F. Fornasiero, H.G. Park, J.K. Holt, M. Stadermann, C.P. Grigoropoulos, A. Noy, O. Bakajin, Ion exclusion by sub-2-nm carbon nanotube pores, Proc. Natl. Acad. Sci. U. S. A. 105 (45) (2008) 17250–17255.  X. Zhao, Y. Liu, S. Inoue, T. Suzuki, R.O. Jones, Y. Ando, Smallest carbon nanotube is 3 angstrom in diameter, Phys. Rev. Lett. (12) (2004) 92.  M. Carrillo-Tripp, M.L. San-Roma´n, J. Hernandez-Cobos, H. Saint-Martin, I. Ortega-Blake, Ion hydration in nanopores and the molecular basis of selectivity, Biophys. Chem. 124 (3) (2006) 243–250, https://doi.org/ 10.1016/j.bpc.2006.04.012.
 B. Tansel, J. Sager, T. Rector, J. Garland, R.F. Strayer, L. Levine, … J. Bauer, Significance of hydrated radius and hydration shells on ionic permeability during nanofiltration in dead end and cross flow modes, Sep. Purif. Technol. 51 (1) (2006) 40–47, https://doi.org/10.1016/j.seppur.2005.12.020.  J.S. Bunch, S.S. Verbridge, J.S. Alden, A.M. van der Zande, J.M. Parpia, H.G. Craighead, P.L. McEuen, Impermeable atomic membranes from graphene sheets, Nano Lett. 8 (2008) 2458–2462.  D.A. Dikin, S. Stankovich, E.J. Zimney, R.D. Piner, G.H.B. Dommett, G. Evmenenko, S.T. Nguyen, R.S. Ruoff, Preparation and characterization of graphene oxide paper, Nature 448 (2007) 457–460.  Y. Zhu, S. Murali, W. Cai, X. Li, J.W. Suk, J.R. Potts, R.S. Ruoff, Graphene and graphene oxide: synthesis, properties, and applications, Adv. Mater. 22 (2010) 3906–3924.  C. Chen, Q.-H. Yang, Y. Yang, W. Lv, Y. Wen, P.-X. Hou, M. Wang, H.-M. Cheng, Self-assembled freestanding graphite oxide membrane, Adv. Mater. 21 (2009) 3007–3011.  R.R. Nair, H.A. Wu, P.N. Jayaram, I.V. Grigorieva, A.K. Gei, Unimpeded permeation of water through helium leak-tight graphene based membranes, Science 335 (6067) (2012) 442–444.  N. Wei, X. Peng, Z. Xu, Understanding water permeation in graphene oxide membranes, Appl. Mater. Interfaces 6 (2014) 5877–5883.  L. Qiu, X. Zhang, W. Yang, Y. Wang, G.P. Simon, D. Li, Controllable corrugation of chemically converted graphene sheet in water and potential application for nanofiltration, Chem. Commun. 47 (2011) 5810–5812.  N.F.D. Aba, J.Y. Chong, B. Wang, C. Mattevi, K. Li, Graphene oxide membranes on ceramic hollow fibers – microstructural stability and nanofiltration performance, J. Membr. Sci. 484 (2015) 87–94, https://doi.org/10.1016/j.memsci.2015.03.001.  K. Goh, L. Setiawan, L. Wei, R. Si, A.G. Fane, R. Wang, Y. Chen, Graphene oxide as effective selective barriers on a hollow fiber membrane for water treatment process, J. Membr. Sci. 474 (2015) 244–253, https://doi.org/10.1016/j.memsci.2014.09.057.  H.M. Hegab, L. Zou, Graphene oxide-assisted membranes: fabrication and potential applications in desalination and water purification, J. Membr. Sci. 484 (2015) 95–106, https://doi.org/10.1016/j.memsci. 2015.03.011.  S. Liu, F. Yao, O. Oderinde, Z. Zhang, G. Fu, Green synthesis of oriented xanthan gum–graphene oxide hybrid aerogels for water purification, Carbohydr. Polym. 174 (2017) 392–399, https://doi.org/10.1016/ j.carbpol.2017.06.044.  M. Hirata, T. Gotou, S. Horiuchi, M. Fujiwara, M. Ohba, Thin-film particles of graphite oxide 1, Carbon 42 (14) (2004) 2929–2937, https://doi.org/10.1016/j.carbon.2004.07.003.  W.S. Hummers Jr., R.E. Offeman, Preparation of graphitic oxide, J. Am. Chem. Soc. 80 (1958) 1133–1339.  D. Li, M.B. M€uller, S. Gilje, R.B. Kaner, G.G. Wallace, Processable aqueous dispersions of graphene nanosheets, Nat. Nanotechnol. 3 (2008) 101–105.  D.R. Dreyer, S. Park, C.W. Bielawski, R.S. Ruoff, The chemistry of graphene oxide, Chem. Soc. Rev. 39 (2010) 228–240.  S. Park, R.S. Ruoff, Chemical methods for the production of graphenes, Nat. Nanotechnol. 4 (2009) 217–224.  H.W. Kim, H. Yoon, S.-M. Yoon, B.M. Yoo, B.K. Ahn, Y.H. Cho, H.J. Shin, H. Yang, U. Paik, S. Kwon, Selective gas transport through few-layered graphene and graphene oxide membranes, Science 342 (2013) 91–95.  H. Li, Z. Song, X. Zhang, Y. Huang, S. Li, Y. Mao, H.J. Ploehn, Y. Bao, M. Yu, Ultrathin, molecular-sieving graphene oxide membranes for selective hydrogen separation, Science 342 (2013) 95–98.  Y.P. Tang, D.R. Paul, T.S. Chung, Free-standing graphene oxide thin films assembled by a pressurized ultrafiltration method for dehydration of ethanol, J. Membr. Sci. 458 (2014) 199–208.  P. Sun, H. Liu, K. Wang, M. Zhong, D. Wu, H. Zhu, Ultrafast liquid water transport through graphene-based nanochannels measured by isotope labelling, Chem. Commun. 51 (2015) 3251–3254.
CHAPTER 14 CARBON NANOTUBE AND GRAPHENE OXIDE
 B. Mi, Graphene oxide membranes for ionic and molecular sieving, Science 343 (2014) 740–742.  S. Pei, H.-M. Cheng, The reduction of graphene oxide, Carbon 50 (9) (2012) 3210–3228, https://doi.org/ 10.1016/j.carbon.2011.11.010.  X. Gao, J. Jang, S. Nagase, Hydrazine and thermal reduction of graphene oxide reaction mechanisms product structures and reaction design, J. Phys. Chem. C 114 (2) (2010) 832–842.  B. Lee, K. Li, H.S. Yoon, J. Yoon, Y.b. Mok, Y. Lee, H.H. Lee, Y.H. Kim, Membrane of functionalized reduced graphene oxide nanoplates with angstrom-level channels, Sci. Rep. (2016) 6.  M.-Y. Lim, Y.-S. Choi, J. Kim, K. Kim, H. Shin, J.-J. Kim, … J.-C. Lee, Cross-linked graphene oxide membrane having high ion selectivity and antibacterial activity prepared using tannic acid-functionalized graphene oxide and polyethyleneimine, J. Membr. Sci. 521 (2017) 1–9, https://doi.org/10.1016/ j.memsci.2016.08.067.  Q. Nan, P. Li, B. Cao, Fabrication of positively charged nanofiltration membrane via the layer-by-layer assembly of graphene oxide and polyethylenimine for desalination, Appl. Surf. Sci. 387 (2016) 521–528, https://doi.org/10.1016/j.apsusc.2016.06.150.  M. Hu, B. Mi, Enabling graphene oxide nanosheets as water separation membranes, Environ. Sci. Technol. 47 (8) (2013) 3715–3723.  Y. Zhang, S. Zhang, T.-S. Chung, Nanometric graphene oxide framework membranes with enhanced heavy metal removal via nanofiltration, Environ. Sci. Technol. 49 (16) (2015) 10235–10242.  G. Zhao, X. Ren, X. Gao, X. Tan, J. Li, C. Chen, Y. Huang, X. Wang, Removal of Pb(II) ions from aqueous solutions on few-layered graphene oxide nanosheets, Dalton Trans. 40 (2011) 10945–10952.  P. Sun, M. Zhu, K. Wang, M. Zhong, J. Wei, D. Wu, X. Zhiping, H. Zhu, Selective ion penetration of graphene oxide membranes, ACS Nano 7 (2013) 428–437.  P. Sun, F. Zheng, M. Zhu, Z. Song, K. Wang, M. Zhong, D. Wu, R.B. Little, Z. Xu, H. Zhu, Selective trans-membrane transport of alkali and alkaline earth cations through graphene oxide membranes based on cation-p interactions, ACS Nano 8 (2014) 850–859.  C.-H. Tsou, Q.-F. An, S.-C. Lo, M. De Guzman, W.-S. Hung, C.-C. Hu, J.-Y. Lai, Effect of microstructure of graphene oxide fabricated through different self-assembly techniques on 1-butanol dehydration, J. Membr. Sci. 477 (2015) 93–100, https://doi.org/10.1016/j.memsci.2014.12.039.  J. Chen, Y. Li, L. Huang, N. Jia, C. Li, G. Shi, Size fractionation of graphene oxide sheets via filtration through track-etched membranes, Adv. Mater. 27 (24) (2015) 3654–3660.  J. Luo, L.J. Cote, V.C. Tung, A.T.L. Tan, P.E. Goins, J. Wu, J. Huang, Graphene oxide nanocolloids, J. Am. Chem. Soc. 132 (50) (2010) 17667–17669.  H. Huang, Z. Song, N. Wei, L. Shi, Y. Mao, Y. Ying, L. Sun, Z. Xu, X. Peng, Ultrafast viscous water flow through nanostrand-channelled graphene oxide membranes, Nat. Commun. 4 (2013).  Y. Ying, L. Sun, Q. Wang, Z. Fan, X. Peng, In-plane mesoporous graphene oxide nanosheet assembled membranes for molecular separation, RCS Adv. 4 (2014) 21425–21428.  W.-S. Hung, Q.-F. An, M. De Guzman, H.-Y. Lin, S.-H. Huang, W.-R. Liu, J.-Y. Lai, Pressure-assisted self-assembly technique for fabricating composite membranes consisting of highly ordered selective laminate layers of amphiphilic graphene oxide, Carbon 68 (2014) 670–677, https://doi.org/10.1016/j.carbon. 2013.11.048.  O.C. Compton, M.J. Palmeri, S.B.T. Nguyen, L.C. Brinson, High-nanofiller-content graphene oxide– polymer nanocomposites via vacuum-assisted self-assembly, Adv. Funct. Mater. 20 (2010) 3322–3329.  K. Huang, G. Liu, J. Shen, Z. Chu, H. Zhou, X. Gu, W. Jin, N. Xu, High efficiency water-transport channels using the synergistic effect of a hydrophilic polymer and graphene oxide laminates, Adv. Funct. Mater. 25 (2015) 5809–5815.  H. Liu, H. Wang, X. Zhang, Facile fabrication of freestanding ultrathin reduced graphene oxide membranes for water purification, Adv. Funct. Mater. 27 (2015) 249–254.  Y. Han, Z. Xu, C. Gao, Ultrathin graphene nanofiltration membrane for water purification, Adv. Funct. Mater. 23 (2013) 3693–3700.
 C.-N. Yeh, K. Raidongia, J. Shao, Q.-H. Yang, J. Huang, On the origin of the stability of graphene oxide membranes in water, Nat. Chem. 7 (2015) 166–170.  J.Y. Chong, N.F.D. Aba, B. Wang, C. Mattevi, K. Li, UV-enhanced sacrificial layer stabilised graphene oxide hollow fibre membranes for nanofiltration, Sci. Rep. (2015) 5.  S.P. Sun, K.Y. Wang, N. Peng, T.A. Hatton, T.-S. Chung, Novel polyamide-imide/cellulose acetate duallayer hollow fiber membranes for nanofiltration, J. Membr. Sci. 363 (1) (2010) 232–242, https://doi.org/ 10.1016/j.memsci.2010.07.038.  P. Marchetti, M.F. Jimenez Solomon, G. Szekely, A.G. Livingston, Molecular separation with organic solvent nanofiltration: a critical review, Chem. Rev. 114 (21) (2014) 10735–10806.  D. An, L. Yang, T.-J. Wang, B. Liu, Separation performance of graphene oxide membrane in aqueous solution, Ind. Eng. Chem. Res. 55 (17) (2016) 4803–4810.  G. Liu, W. Jin, N. Xu, Graphene-based membrane, Chem. Soc. Rev. 44 (15) (2015) 5016–5030. [111a] A.K. Geim, Graphene: status and prospects, Science 324 (5934) (2009) 1530–1534. [111b] J.C. Meyer, A.K. Geim, M.I. Katsnelson, K.S. Novoselov, T.J. Booth, S. Roth, The structure of suspended graphene sheets, Nature 446 (2007) 60–63. [111c] M. Yang, C. Zhao, S. Zhang, P. Li, D. Hou, Preparation of graphene oxide modified poly(m-phenylene isophthalamide) nanofiltration membrane with improved water flux and antifouling property, Appl. Surface Sci 394 (Suppl C) (2017) 149–159.  B.J. Hinds, N. Chopra, T. Rantell, R. Andrews, V. Gavalas, L.G. Bachas, Aligned multiwalled carbon nanotube membranes, Science 303 (5654) (2004) 62–65.  S. Li, H. Li, X. Wang, Y. Song, Y. Liu, L. Jiang, D. Zhu, Super hydrophobicity of large area honeycomb like aligned carbon nanotubes, J. Phys. Chem. B 106 (36) (2002) 9274–9276.  D. Cohen-Tanugi, J.C. Grossman, Water desalination across nanoporous graphene, Nano Lett. 12 (7) (2012) 3602–3608.  E.A. M€uller, Purification of water through nanoporous carbon membranes: a molecular simulation viewpoint, Curr. Opin. Chem. Eng. 2 (2) (2013) 223–228, https://doi.org/10.1016/j.coche.2013.02.004.  W.-F. Chan, H.-Y. Chen, A. Surapathi, M.G. Taylor, X. Shao, E. Marand, J.K. Johnson, Zwitterion functionalized carbon nanotube/polyamide nanocomposite membranes for water desalination, ACS Nano 7 (6) (2013) 5308–5319.  T.V. Ratto, J.K. Holt, A.W. Szmodis, G. patents, 2011.  M. Mulder, Basic Principles of Membrane Technology, second ed, Kluwer Academic Publisher, London, 1996.  B. Van der Bruggen, M. M€antt€ari, M. Nystr€ om, Drawbacks of applying nanofiltration and how to avoid them: a review, Sep. Purif. Technol. 63 (2) (2008) 251–263, https://doi.org/10.1016/j.seppur.2008.05.010.  M. Majumder, N. Chopra, B.J. Hinds, Mass transport through carbon nanotube membranes in three different regimes: ionic diffusion and gas and liquid flow, ACS Nano 5 (2011) 3867–3877.  S. Karan, S. Samitsu, X. Peng, K. Kurashima, I. Ichinose, Ultrafast viscous permeation of organic solvents through diamond like carbon nanosheets, Science 335 (2012) 444–447.  D.R. Paul, Creating new types of carbon-based membranes, Science 335 (2012) 413–414.  D. Krishnan, F. Kim, J. Luo, R. Cruz-Silva, L.J. Cote, H.D. Jang, J. Huang, Energetic graphene oxide: challenges and opportunities, Nano Today 7 (2) (2012) 137–152, https://doi.org/10.1016/j.nantod.2012.02.003.  R.K. Joshi, P. Carbone, F.C. Wang, V.G. Kravets, Y. Su, I.V. Grigorieva, H.A. Wu, A.K. Geim, R.R. Nair, Precise and ultrafast molecular sieving through graphene oxide membrane, Sci. Rep. 343 (6172) (2014) 752–754.  K. Raidongia, J. Huang, Nanofluidic ion transport through reconstructed layered materials, J. Am. Chem. Soc. 134 (2012) 16528–16531.